Magnetostriction (cf. electrostriction) is a property of ferromagnetic materials that causes them to change their shape or dimensions during the process of magnetization. The variation of materials's magnetization due to the applied magnetic field changes the magnetostrictive strain until reaching its saturation value, λ. The effect was first identified in 1842 by James Joule when observing a sample of iron.
This effect causes losses due to frictional heating in susceptible ferromagnetic cores. The effect is also responsible for the low-pitched humming sound that can be heard coming from transformers.
Internally, ferromagnetic materials have a structure that is divided into domains, each of which is a region of uniform magnetic polarization. When a magnetic field is applied, the boundaries between the domains shift and the domains rotate; both of these effects cause a change in the material's dimensions.
The reciprocal effect, the change of the susceptibility (response to an applied field) of a material when subjected to a mechanical stress, is called the Villari effect. Two other effects are thus related to magnetostriction: the Matteucci effect is the creation of a helical anisotropy of the susceptibility of a magnetostrictive material when subjected to a torque and the Wiedemann effect is the twisting of these materials when a helical magnetic field is applied to them.
The Villari reversal is the change in sign of the magnetostriction of iron from positive to negative when exposed to magnetic fields of approximately 40,000 A/m.
On magnetization, a magnetic material undergoes changes in volume which are small: of the order 10−6.
Magnetostrictive hysteresis loop
Like flux density, the magnetostriction also exhibit hysteresis versus strength of magnetizing field. The shape of this hysteresis loop (called "butterfly loop") can be reproduced using the Jiles-Atherton model.
Magnetostrictive materials can convert magnetic energy into kinetic energy, or the reverse, and are used to build actuators and sensors. The property can be quantified by the magnetostrictive coefficient, Λ, which may be positive or negative and is defined as the fractional change in length as the magnetization of the material increases from zero to the saturation value. The effect is responsible for the familiar "electric hum" ( Listen (help·info)) which can be heard near transformers and high power electrical devices.
Cobalt exhibits the largest room-temperature magnetostriction of a pure element at 60 microstrains. Among alloys, the highest known magnetostriction is exhibited by Terfenol-D, (Ter for terbium, Fe for iron, NOL for Naval Ordnance Laboratory, and D for dysprosium). Terfenol-D, TbxDy1-xFe2, exhibits about 2,000 microstrains in a field of 2 kOe (160 kA/m) at room temperature and is the most commonly used engineering magnetostrictive material.
Another very common magnetostrictive composite is the amorphous alloy Fe81Si3.5B13.5C2 with its trade name Metglas 2605SC. Favourable properties of this material are its high saturation-magnetostriction constant, λ, of about 20 microstrains and more, coupled with a low magnetic-anisotropy field strength, HA, of less than 1 kA/m (to reach magnetic saturation). Metglas 2605SC also exhibits a very strong ΔE-effect with reductions in the effective Young's modulus up to about 80% in bulk. This helps build energy-efficient magnetic MEMS.
- Coil noise
- Inverse magnetostrictive effect
- FeONIC—developer of audio products using magnetostriction
- Joule, J.P. (1847). "On the Effects of Magnetism upon the Dimensions of Iron and Steel Bars". The London, Edinburgh and Dublin philosophical magazine and journal of science (Taylor & Francis). 30, Third Series: 76–87, 225–241. Retrieved 2009-07-19. Joule observed in this paper that he first reported the measurements in a "Conversazione" in Manchester, England, in Joule, James (1842). "On a new class of magnetic forces". Annals of Electricity, Magnetism, and Chemistry 8: 219–224.
- Questions & answers on everyday scientific phenomena. Sctritonscience.com. Retrieved on 2012-08-11.
- Szewczyk, R. (2006). "Modelling of the magnetic and magnetostrictive properties of high permeability Mn-Zn ferrites". PRAMANA-Journal of Physics 67 (6): 1165. doi:10.1007/s12043-006-0031-z.
- "Magnetostriction and Magnetostrictive Materials". Active Material Laboratory. UCLA. Archived from the original on 2006-02-02.
- "Magnetostriction and transformer noise". Archived from the original on 2006-05-10.
- Invisible Speakers from Feonic that use Magnetostriction